Application of Graphene Silicone Grease in heat dissipation for the
Intel Core i5 Processor
Mai Thi Phuong#*
, Bui Anh Tuan#
, Trần Văn Hậu#*
, Pham Van Trinh#
, Nguyen Nang Dinh*
Phan Ngoc Minh**
, Bui Hung Thang#
Institute of Materials Science, Vietnam Academy of Science and Technology, Hanoi, Vietnam
VNU University of Engineering and Technology, Ha Noi, Vietnam
Graduate University of Science and Technology, Vietnam Academy of Science and Technology, Hanoi, Vietnam
Abstract— Graphene was known as the material that owning many superiority properties and high thermal conductivity. Thermal
conductivity of single-layer graphene was up to 5200 W/mK (compared to the thermal conductivity of Carbon nanotubes 2000 W/mK
and Silver 410 W/mK). This had suggested that graphene is the most potential material for heat dissipation applications for electronic
devices, such as a computer microprocessor, high power LED... To enhance the dispersion of the GNPs silicone matrix, we were
functionalized graphene nanoplatelets (GNPs) with carboxyl (-COOH) groups. The silicone thermal greases containing GNPs were
prepared by High- Energy Ball Milling method (8000D Mixer /Mill). The results of SEM, FTIR, Raman showed the presence of the
carboxyl groups in GNPs and GNPs uniform dispersion dispersed in grease. The results of thermal conductivity from Transient Hot
Bridge THB-100 showed that thermal conductivity enhancement was up to 234 % with Gr-COOH 1.0 vol.%. Thermal grease is used
as a thermal interface material to coolants for Intel Core i5 processor. The results of thermal dissipation efficiency shown the
saturation temperature of the processor using thermal grease containing 1.0 vol.% Gr-COOH decreased 4℃, compared to the silicone
Keywords— thermal grease, silicone grease, graphene, CPU, Intel Core i5 processor.
Nowadays, the process of miniaturization with the
development of high-power electronic devices and
manufacturing processes developed at the nanometer-level.
The electronic devices allow higher transistor integration
density in the processor (CPU) [1-4]. However, computer
processors action for a long will consume energy and release
large amounts of heat. The excessive amount of heat
generated will reduce the lifespan, reliability and efficiency
of the CPU because the electronic devices only work into a
certain temperature limit . Therefore, the heat generated
from high-power electronic devices should be dissipated as
quickly and effectively as possible, to maintain the operating
temperatures of the devices at the desired level. In the way
stated, the heat dissipation enhancement has become one of
the most crucial issues that raise the reliability, boosts
performance and stability of high-power electronic devices
such as microprocessors, and especially is Central
Processing Unit (CPU) [6,7].
Current cooling methods are only reaching a certain limit
due to the interface area between CPU and heatsink [8,9].
Therefore, the use of thermal grease in high-power
electronic devices of great interest by researchers and
manufacturers. Thermal grease is a typical thermal interface
material (TIM) , usually used to increase the thermal
conductivity between microprocessors and heat sinks .
The main materials of thermal grease consist of the matrix
polymer and filler [12,13]. The filler materials are key
thermal conductivity ingredient in silicone thermal grease. It
is sized particles µm with high thermal conductivity and
dispersed in the base silicone, often use inorganic or metal
nanomaterials with high thermal conductivity [14-18].
Thermal silicon grease fills the gaps between two solid
surfaces and establishes an efficient heat path, thereby
enhancing thermal conductivity [19-21]. The thermal
conductivity of fat increases with increasing filler content.
However, many factors have an effect on thermal
conductivity of grease, such as the size of particles, the
particle dispersion in base grease, and the thermal properties
of the dispersed particle [22,23]. In recent years, many
thermal greases have been reported using nanomaterials with
high conductivity for better performance. Researchers have
recently shown much interest in the issue of finding new
INTERNATIONAL JOURNAL ON INFORMATICS VISUALIZATION
VOL 3 (2019) NO 2-2
e-ISSN : 2549-9904
ISSN : 2549-9610
materials for thermal grease in the heat dissipation future
Recently, Graphene is a two-dimensional nanocarbon
material with the hexagonally packed structure compromised
of sp2-hybridized carbon atoms, discovered by Andre Geim
and Kostya Novoselov in 2004 . Baladin et al.’s research
showed that the in-plane thermal conductivity of single-layer
graphene was up to 5200 W/mK  (compared to the
thermal conductivity of CNTs 2000 W/mK and Ag 410
W/mK) . This suggests an approach in applying
graphene in grease or liquid for thermal dissipation systems
for computer processors and other high-power electronic
In this paper, we report on the new results in the
fabrication of high thermal conductivity silicone grease
containing graphene, and application grease for enhancing
heat dissipation of Intel Core i5 processor .
II. THE MATERIAL AND METHOD
The graphene nanoplatelets materials (GNPs) were
purchased from ACS Material Company with a purity of
99.5%, thickness 20 nm, diameter 5-10 μm, density 2,3
, and specific surface area 20-40 m2
/g. GNPs was
functionalized by treatment with a mixture HNO3 and
H2SO4 acids at a ratio of 1:3 (v/v) at a temperature of 70℃
for 5h to form a carboxyl (-COOH) group, as schematically
shown in Figure 1. Raman spectroscopy was used to analyze
graphitic change the graphene materials after acid treatment.
Chemical bonds and elements in thermal grease were
characterized by Fourier-transform infrared spectroscopy
Fig.1. The creative process of graphene functionalized by carboxyl (-
In order to disperse the Gr-COOH in the silicone grease,
we using by 8000D Mixer /Mill (High- Energy Ball Mill) at
a speed of 8000 rpm for 3 hours. Field-emission scanning
electron microscope (FESEM) was used to examine the size,
morphology, and distribution of Gr-COOH in the thermal
grease. Thermal conductivity of the grease is measured by
Transient Hot Bridge THB-100 (Linseis, Germany) at room
temperature. Figure 2 is a schematic view of the thermal
dissipation system for a computer processor using silicone
grease containing Gr-COOH. In this model, thermal grease
was painted on the interface between the CPU chip and the
heatsink. We use the air conditioner to keep the ambient
temperature at 28◦C for all measurements. Thermal grease
replaces the air gap with thermal conductivity of 0.026
W/m.K and fills the gap between the rugged surface and the
heat path setting, thereby increasing the heat transfer
efficiency. The thermal dissipation efficiency was evaluated
by using dedicated software and built-in temperature sensors
inside the microprocessor to measure the temperature of the
The computer used in this study has the following
configuration: Intel Core i5 – 3570 K Processor, Corsair’s 4
GB DDR3 SODIMM Memory, Toshiba’s 1 TB Hard Disk
Drive, Asrock H61M-VS3 Mainboard, and Window 10
Ultimate Service Pack 1 Operating System for all
experiments. The temperature of the microprocessor was
measured by using the Core Temp 1.10.2- 64 bit software.
The microprocessor was pushed to the maximum (100%
usage of the processor) by using Prime95 32 bit 29.3 build 1
Fig.2. Scheme of the cooling system using thermal grease containing Gr-
III. RESULTS AND DISCUSSION
Figure 3 shows a typical FESEM image of the GNPs
hight magnification. The thickness of nanosheets in the
range of 2–10 nm, the average diameter was about 5-10 µm
with high cleanliness and purity 99%.
Fig.3. FESEM image of graphene nanoplatelets
Raman scattering is a technique to examine the changes
in the surfaces and the structures of GNPs. Figure 4 clearly
shows that the G band (around 1582.87) and 2D band
(around 2678.2). The D-band intensity was appeared in the
functionalized GNPs compared to the pristine GNPs. The
intensity ratio of D lines to G lines was different, suggesting
some changes in the surfaces and the structures of the GNPs.
This result indicates that some of the sp2
(C=C) were converted to sp3
carbon atoms (C−C) at the
surfaces of the MWCNTs after the acid treatment in
Fig.4. Raman spectra of Graphene (red line), Gr-COOH (blue line)
Figure 5 presents the typical FTIR spectra of the pristine
GNPs and Gr-COOH. Some important peaks are seen after
the GNPs have been treated with a mixture of H2SO4 and
HNO3. The vibration of O-H bonding in the carboxyl group
is shown as a peak at 3446 cm-1
. It was expanded more than
that of the O-H bonding of H2O. The peak at 1708 cm-1
showed the existence of vibrations of the C=O bond in the
carboxyl group. This shows the importance of proving the
existence of carboxyl (COOH) functional groups due to the
oxidation resulting from the nitric and the sulfuric acids.
This clearly shows that the acids functionalized the surfaces
of the GNPs.
Fig.5. FTIR transmission spectra of pristine GNPs, Gr-COOH.
Fig. 6a shows the SEM images of silicone thermal grease.
As can be seen, the silicone thermal grease used in this
research contains some large and small filling particles
inequitably distributed in the grease. Fig. 6b shows the SEM
images of thermal grease containing 1.0 vol.% Gr-COOH as
prepared. This result shows the distribution of the metal
oxide particles of the grease and Gr-COOH inside thermal
grease after annealing. This indicates that silicone grease
clings to graphene. In other words, Gr-COOH were good
compatibility and well-dispersed in the silicone grease,
thereby enhancing the thermal conductivity of grease.
Fig.6. FESEM image of silicone thermal grease (a) and silicone thermal
grease containing Gr-COOH (b)
THE RESULT THERMAL CONDUCTVITY OF THE GREASE
Thermal conductivity of grease containing GNP
0.75 vol.% 1.0 vol.%
(k-k0)/k0 74% 130% 171% 234%
The statistic results of thermal conductivity and the
thermal conductivity enhancement of thermal grease with
different Gr-COOH concentration are reported in table 1. In
which, k and k0 are the thermal conductivity of the silicone
thermal grease and the thermal grease containing Gr-COOH,
respectively. The equations (k−k0)/k0 shown the thermal
conductivity enhancement. The result shows with 0.25, 0.5,
0.75 and 1 vol.% Gr-COOH the thermal conductivity of
thermal grease containing Gr-COOH was measured to be
3.210, 4.281, 5.012, 6.172 W/m.K. Similarly, the thermal
conductivity enhancement was calculated to be 74%, 130%,
171%, 234% corresponding to the thermal grease containing
0.25, 0.5, 0.75 and 1.0 vol.%, respectively. Results showed
that Gr-COOH 1.0 vol.% had the highest thermal
conductivity enhancement of 234% compared with silicone
Fig.7. The measured temperature of the microprocessor as a function of the
operation time in the case of using thermal grease
The temperature microprocessor of the can be measured
directly when it during the operation of the computer at full
load mode. We use an air conditioner to kept well room
temperature at 28℃ for all measurements. We use thermal
grease to reduce the saturation temperature and slow down
the temperature increase of the processor. Figure 7 shows the
microprocessor's experimental temperature as a function of
working time when using thermal grease. At the initial time,
the temperature of the microprocessor was about 32℃, after
about 240 seconds the temperature reached saturation. The
saturation temperature of the microprocessor reached 62℃
when using silicone thermal grease and it reached 61℃,
60℃, 59℃, 58℃ with silicone thermal grease containing
Gr-COOH with 0.25 vol.%, 0.5 vol.%, 0.75% vol.%, 1
vol.%, respectively. Similarly, the saturation temperature
decrease of CPU was calculated to be 1, 2, 3, 4
correspondings to the thermal grease containing 0.25, 0.5,
0.75 and 1.0 vol.%, responding. The lowest saturation
temperature of CPU was 58℃ with grease containing 1
The successful functionalization Gr-COOH by a mixture
of the acid solution was proven by Raman and FTIR spectral
measurements. The SEM images proved that graphene
nanoplatelets dispersed in the based grease by high energy
ball mill method. The results thermal conductivity from
Transient Hot Bridge THB-100 showed that thermal
conductivity enhancement was up to 234 % with Gr-COOH
1.0 vol.%. The thermal dissipation efficiency of the PC’s
microprocessor examined and evaluated. Compared to the
silicone grease, the saturation temperature of the processor
using thermal grease containing 1.0 vol.% Gr-COOH
decreased 4 ℃ . The obtained results confirmed the
advantages of using Gr-COOH for thermal grease in
microprocessors and other high-power electronic devices.
This study was funded from: “For Inspiration and
Recognition of Science and Technology (FIRST) under
  P. K. Schelling, L. Shi, and K. E. Goodson, “Managing heat for
electronics,” Mater. Today, vol. 8, no. 6, pp. 30–35, Jun. 2005.
  K. M. Razeeb, E. Dalton, G. L. W. Cross, and A. J. Robinson,
“Present and future thermal interface materials for electronic
devices,” Int. Mater. Rev., vol. 63, no. 1, pp. 1–21, Jan. 2018.
  N. T. Hong, K. H. Koh, N. T. T. Tam, P. N. Minh, P. H. Khoi,
and S. Lee, “Combined model for growing mechanism of carbon
nanotubes using HFCVD: effect of temperature and molecule gas
diffusion,” Thin Solid Films, vol. 517, no. 12, pp. 3562–3565, Apr.
  B. Hung Thang, P. Van Trinh, N. Van Chuc, P. H. Khoi, and P.
N. Minh, “Heat Dissipation for Microprocessor Using Multiwalled
Carbon Nanotubes Based Liquid,” Sci. World J., vol. 2013, pp. 1–6,
  J. Falck, C. Felgemacher, A. Rojko, M. Liserre, and P. Zacharias,
“Reliability of Power Electronic Systems: An Industry Perspective,”
IEEE Ind. Electron. Mag., vol. 12, no. 2, pp. 24–35, Jun. 2018.
  Y. Song and B. Wang, “Survey on Reliability of Power
Electronic Systems,” IEEE Trans. Power Electron., vol. 28, no. 1, pp.
591–604, Jan. 2013.
  F. L. Tan and C. P. Tso, “Cooling of mobile electronic devices
using phase change materials,” Appl. Therm. Eng., vol. 24, no. 2–3,
pp. 159–169, Feb. 2004.
  R. L. Webb and J. P. Gwinn, “Low melting point thermal
interface material,” in ITherm 2002. Eighth Intersociety Conference
on Thermal and Thermomechanical Phenomena in Electronic
Systems (Cat. No.02CH37258), pp. 671–676.
  D. D. L. Chung, “Thermal Interface Materials,” J. Mater. Eng.
Perform., vol. 10, no. 1, pp. 56–59, Feb. 2001.
 F. Sarvar, D. Whalley, and P. Conway, “Thermal Interface
Materials - A Review of the State of the Art,” in 2006 1st Electronic
Systemintegration Technology Conference, 2006, pp. 1292–1302.
 J. Due and A. J. Robinson, “Reliability of thermal interface
materials: A review,” Appl. Therm. Eng., vol. 50, no. 1, pp. 455–463,
 S. Yeol Jeong and Y. Suk Choi, “Measurement of interfacial
thermal resistance of silicone based grease in wide temperature range
by laser flash method,” High Temp. Press., vol. 48, no. 1–2, p. 59,
 M. A. Vadivelu, C. R. Kumar, and G. M. Joshi, “Polymer
composites for thermal management: a review,” Compos. Interfaces,
vol. 23, no. 9, pp. 847–872, Nov. 2016.
 D. D. . Chung, “Materials for thermal conduction,” Appl. Therm.
Eng., vol. 21, no. 16, pp. 1593–1605, Nov. 2001.
 H. Chen, H. Wei, M. Chen, F. Meng, H. Li, and Q. Li,
“Enhancing the effectiveness of silicone thermal grease by the
addition of functionalized carbon nanotubes,” Appl. Surf. Sci., vol.
283, pp. 525–531, Oct. 2013.
 W. Zhou, S. Qi, C. Tu, H. Zhao, C. Wang, and J. Kou, “Effect of
the particle size of Al2O3 on the properties of filled heat-conductive
silicone rubber,” J. Appl. Polym. Sci., vol. 104, no. 2, pp. 1312–1318,
 Q. Wang, W. Gao, and Z. Xie, “Highly thermally conductive
room-temperature-vulcanized silicone rubber and silicone grease,” J.
Appl. Polym. Sci., vol. 89, no. 9, pp. 2397–2399, Aug. 2003.
 W. Yu, H. Xie, L. Yin, J. Zhao, L. Xia, and L. Chen,
“Exceptionally high thermal conductivity of thermal grease:
Synergistic effects of graphene and alumina,” Int. J. Therm. Sci., vol.
91, pp. 76–82, May 2015.
 J. Hansson, T. M. J. Nilsson, L. Ye, and J. Liu, “Novel
nanostructured thermal interface materials: a review,” Int. Mater.
Rev., vol. 63, no. 1, pp. 22–45, Jan. 2018.
 U. Eduok, O. Faye, and J. Szpunar, “Recent developments and
applications of protective silicone coatings: A review of PDMS
functional materials,” Prog. Org. Coatings, vol. 111, pp. 124–163,
 L. Calabrese, L. Bonaccorsi, A. Freni, and E. Proverbio,
“Silicone composite foams for adsorption heat pump applications,”
Sustain. Mater. Technol., vol. 12, pp. 27–34, Jul. 2017.
 N. Burger, A. Laachachi, M. Ferriol, M. Lutz, V. Toniazzo, and
D. Ruch, “Review of thermal conductivity in composites:
Mechanisms, parameters and theory,” Prog. Polym. Sci., vol. 61, pp.
1–28, Oct. 2016.
 S. Zhai, P. Zhang, Y. Xian, J. Zeng, and B. Shi, “Effective
thermal conductivity of polymer composites: Theoretical models and
simulation models,” Int. J. Heat Mass Transf., vol. 117, pp. 358–374,
 P. Zhang, J. Zeng, S. Zhai, Y. Xian, D. Yang, and Q. Li,
“Thermal Properties of Graphene Filled Polymer Composite Thermal
Interface Materials,” Macromol. Mater. Eng., vol. 302, no. 9, p.
1700068, Sep. 2017.
 H. Chen et al., “Thermal conductivity of polymer-based
composites: Fundamentals and applications,” Prog. Polym. Sci., vol.
59, pp. 41–85, Aug. 2016.
 K. S. Novoselov, “Electric Field Effect in Atomically Thin
Carbon Films,” Science (80-. )., vol. 306, no. 5696, pp. 666–669, Oct.
 A. A. Balandin et al., “Superior Thermal Conductivity of Single-
Layer Graphene,” Nano Lett., vol. 8, no. 3, pp. 902–907, Mar. 2008.
 H. T. Bui, V. C. Nguyen, V. T. Pham, T. T. T. Ngo, and N. M.
Phan, “Thermal dissipation media for high power electronic devices
using a carbon nanotube-based composite,” Adv. Nat. Sci. Nanosci.
Nanotechnol., vol. 2, no. 2, p. 025002, Apr. 2011.
 B. H. Thang, P. Van Trinh, L. D. Quang, N. T. Huong, P. H.
Khoi, and P. N. Minh, “Heat dissipation for the Intel Core i5
processor using multiwalled carbon-nanotube-based ethylene
glycol,” J. Korean Phys. Soc., vol. 65, no. 3, pp. 312–316, 2014.